LMucko/crystallography-open-database huggingface dataset:
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222425
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           ?
_space_group_ssg_name            C21/m1(\a\b0)0ss
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  ?
_symmetry_space_group_name_H-M   ?
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.262(3)
_cell_formula_units_Z            2
_cell_length_a                   6.8939(3)
_cell_length_b                   11.9135(5)
_cell_length_c                   4.80731(5)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     394.82(2)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0183
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0374
_pd_proc_ls_prof_wR_expected     0.0069
_pd_proc_ls_prof_wR_factor       0.0415
_refine_ls_number_constraints    0
_refine_ls_number_parameters     66
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0483
_refine_ls_shift/su_mean         0.0080
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Ia
_cod_original_cell_volume        394.83(2)
_cod_database_code               7222425
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222426
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           ?
_space_group_ssg_name            C21/m1(\a\b0)0ss
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  ?
_symmetry_space_group_name_H-M   ?
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.222(3)
_cell_formula_units_Z            2
_cell_length_a                   6.8929(3)
_cell_length_b                   11.9152(5)
_cell_length_c                   4.80610(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     394.72(2)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0191
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0372
_pd_proc_ls_prof_wR_expected     0.0069
_pd_proc_ls_prof_wR_factor       0.0400
_refine_ls_number_constraints    0
_refine_ls_number_parameters     66
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0421
_refine_ls_shift/su_mean         0.0065
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Id
_cod_database_code               7222426
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222427
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           ?
_space_group_ssg_name            C21/m1(\a\b0)0ss
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  ?
_symmetry_space_group_name_H-M   ?
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.222(3)
_cell_formula_units_Z            2
_cell_length_a                   6.8929(3)
_cell_length_b                   11.9152(5)
_cell_length_c                   4.80610(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     394.72(2)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0191
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0372
_pd_proc_ls_prof_wR_expected     0.0069
_pd_proc_ls_prof_wR_factor       0.0400
_refine_ls_number_constraints    0
_refine_ls_number_parameters     66
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0421
_refine_ls_shift/su_mean         0.0065
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Ic
_cod_database_code               7222427
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
_cod_duplicate_entry 7222426
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222428
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           ?
_space_group_ssg_name            C21/m1(\a\b0)0ss
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  ?
_symmetry_space_group_name_H-M   ?
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90.200(3)
_cell_formula_units_Z            2
_cell_length_a                   6.8924(3)
_cell_length_b                   11.9164(5)
_cell_length_c                   4.80483(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     394.63(2)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0198
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0362
_pd_proc_ls_prof_wR_expected     0.0070
_pd_proc_ls_prof_wR_factor       0.0383
_refine_ls_number_constraints    0
_refine_ls_number_parameters     66
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0481
_refine_ls_shift/su_mean         0.0020
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Ie
_cod_original_cell_volume        394.63(3)
_cod_database_code               7222428
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222429
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           63
_space_group_ssg_name            Ccmm1(0\b0)00ss
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2c'
_symmetry_space_group_name_H-M   'C c m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.90396(6)
_cell_length_b                   11.89561(11)
_cell_length_c                   4.79590(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     393.872(6)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0256
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0331
_pd_proc_ls_prof_wR_expected     0.0069
_pd_proc_ls_prof_wR_factor       0.0336
_refine_ls_number_constraints    0
_refine_ls_number_parameters     51
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0320
_refine_ls_shift/su_mean         0.0022
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           If
_cod_original_cell_volume        393.873(6)
_cod_database_code               7222429
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222430
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           63
_space_group_ssg_name            Ccmm1(0\b0)00ss
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2c'
_symmetry_space_group_name_H-M   'C c m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.90198(6)
_cell_length_b                   11.90062(11)
_cell_length_c                   4.79640(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     393.966(6)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0249
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_pd_proc_ls_prof_R_factor        0.0326
_pd_proc_ls_prof_wR_expected     0.0069
_pd_proc_ls_prof_wR_factor       0.0335
_refine_ls_number_constraints    0
_refine_ls_number_parameters     51
_refine_ls_number_restraints     0
_refine_ls_shift/su_max          0.0457
_refine_ls_shift/su_mean         0.0060
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Ig
_cod_database_code               7222430
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric effect material
Gottschilch, Michael; Gourdon, Olivier; Persson, Joerg; de la Cruz, Clarina; Petricek, Vaclav; Brueckel, Thomas; Journal of Materials Chemistry 22 (2012) 15275–; doi:10.1039/c2jm00154c

data_7222431
_publ_section_title
;
 Study of the antiferromagnetism of Mn5Si3: an inverse magnetocaloric
 effect material
;
_journal_issue                   30
_journal_name_full               'Journal of Materials Chemistry'
_journal_page_first              15275
_journal_paper_doi               10.1039/c2jm00154c
_journal_volume                  22
_journal_year                    2012
_chemical_absolute_configuration .
_chemical_formula_sum            'Mn5 Si3'
_chemical_formula_weight         358.9
_chemical_name_systematic        ' ?'
_space_group_IT_number           63
_space_group_ssg_name            Ccmm1(0\b0)00ss
_symmetry_cell_setting           orthorhombic
_symmetry_space_group_name_Hall  '-C 2c 2c'
_symmetry_space_group_name_H-M   'C c m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   6.89900(7)
_cell_length_b                   11.90799(11)
_cell_length_c                   4.79730(4)
_cell_measurement_temperature    90
_cell_modulation_dimension       1
_cell_volume                     394.114(6)
_diffrn_ambient_temperature      90
_diffrn_radiation_type           neutron
_diffrn_radiation_wavelength     -1
_exptl_absorpt_coefficient_mu    0
_exptl_crystal_density_diffrn    3.0238
_exptl_crystal_F_000             668
_pd_instr_location               ' ?'
_pd_meas_2theta_range_max        72.793
_pd_meas_2theta_range_min        7.006
_pd_meas_number_of_points        2343
_pd_proc_2theta_range_max        72.793
_pd_proc_2theta_range_min        7.006
_pd_proc_ls_background_function  '10 Legendre polynoms'
_pd_proc_ls_pref_orient_corr     none
_pd_proc_ls_profile_function     Gaussian
_refine_ls_number_constraints    0
_refine_ls_number_restraints     0
_refine_ls_weighting_scheme      sigma
_cod_data_source_file            c2jm00154c.txt
_cod_data_source_block           Ih
_cod_database_code               7222431
_jana_cell_commen_supercell_matrix_1_1 1
_jana_cell_commen_supercell_matrix_1_2 0
_jana_cell_commen_supercell_matrix_1_3 0
_jana_cell_commen_supercell_matrix_2_1 0
_jana_cell_commen_supercell_matrix_2_2 1
_jana_cell_commen_supercell_matrix_2_3 0
_jana_cell_commen_supercell_matrix_3_1 0
_jana_cell_commen_supercell_matrix_3_2 0
_jana_cell_commen_supercell_matrix_3_3 1
_jana_cell_commen_t_section_1    0
Control of the properties of magnetic ferrite-alloys using the ions Al3+, Cr3+, Sc3+, In3+
Kirichok, P.P.; Antoshchuk, A.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 13 (1977) 1327–1330; doi:

data_1533906
_publ_section_title
;
 Control of the properties of magnetic ferrite-alloys using the ions Al3+,
 Cr3+, Sc3+, In3+
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              1327
_journal_page_last               1330
_journal_volume                  13
_journal_year                    1977
_chemical_formula_sum            'Al0.2 Fe1.8 Mg O4'
_chemical_name_systematic        'Mg Al.2 Fe1.8 O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.359
_cell_length_b                   8.359
_cell_length_c                   8.359
_cell_volume                     584.067
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Kirichok_IVNMAW_1977_1635.cif
_cod_data_source_block           Al0.2Fe1.8Mg1O4
_cod_original_cell_volume        584.0674
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Al0.2 Fe1.8 Mg1 O4'
_cod_database_code               1533906
Pressure-temperature phase diagram of Se O2. Characterization of new phases
Orosel, D.; Leynaud, O.; Balog, P.; Jansen, M.; Journal of Solid State Chemistry 177 (2004) 1631–1638; doi:

data_1533907
_publ_section_title
;
 Pressure-temperature phase diagram of Se O2. Characterization of new
 phases
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              1631
_journal_page_last               1638
_journal_volume                  177
_journal_year                    2004
_chemical_formula_sum            'O2 Se'
_chemical_name_systematic        'Se O2'
_space_group_IT_number           26
_symmetry_space_group_name_Hall  'P 2c -2'
_symmetry_space_group_name_H-M   'P m c 21'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.0722
_cell_length_b                   4.4704
_cell_length_c                   7.5309
_cell_volume                     170.761
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Orosel_JSSCBI_2004_1687.cif
_cod_data_source_block           O2Se1
_cod_original_cell_volume        170.7614
_cod_original_formula_sum        'O2 Se1'
_cod_database_code               1533907
Control of the properties of magnetic ferrite-alloys using the ions Al3+, Cr3+, Sc3+, In3+
Kirichok, P.P.; Antoshchuk, A.P.; Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy 13 (1977) 1327–1330; doi:

data_1533908
_publ_section_title
;
 Control of the properties of magnetic ferrite-alloys using the ions Al3+,
 Cr3+, Sc3+, In3+
;
_journal_name_full
'Izvestiya Akademii Nauk SSSR, Neorganicheskie Materialy'
_journal_page_first              1327
_journal_page_last               1330
_journal_volume                  13
_journal_year                    1977
_chemical_formula_sum            'Al0.6 Fe1.4 Mg O4'
_chemical_name_systematic        'Mg Al.6 Fe1.4 O4'
_space_group_IT_number           227
_symmetry_space_group_name_Hall  'F 4d 2 3 -1d'
_symmetry_space_group_name_H-M   'F d -3 m :1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   8.326
_cell_length_b                   8.326
_cell_length_c                   8.326
_cell_volume                     577.177
_citation_journal_id_ASTM        IVNMAW
_cod_data_source_file            Kirichok_IVNMAW_1977_1644.cif
_cod_data_source_block           Al0.6Fe1.4Mg1O4
_cod_original_cell_volume        577.1773
_cod_original_sg_symbol_Hall     '-F 4vw 2vw 3 (x+1/8,y+1/8,z+1/8)'
_cod_original_formula_sum        'Al0.6 Fe1.4 Mg1 O4'
_cod_database_code               1533908